SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715 MeasuringSupplementary Informationnonlinear to stresses “Measuring generated Nonlinear Stresses by Generateddefects by in Defects 3D colloidal in 3D Colloidal crystals Crystals” 1 1 2 1 1 Neil Y.C. Lin†, Matthew Bierbaum†, Peter Schall, James P. Sethna, and Itai Cohen

1Department of Physics, Cornell University, Ithaca, NY 14853 2Institute of Physics, University of Amsterdam, Amsterdam, The Netherlands

† These authors contributed equally to this work

NATURE MATERIALS | www.nature.com/naturematerials 1 © 2016 Macmillan Publishers1 Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

Contents

I. Derivation of the SALSA method 3 A. Derivation 3 B. Local structural anisotropy tensor 4 C. From pointwise functions to continuum ﬁelds 5

II. Calibration of the SALSA method 9 A. Calibration: SALSA versus actual stress 10 B. Calibration: Contact criteria dependence 10 C. Calibration: Mechanical equilibrium of a smoothed ﬁeld 14

III. Vacancy Stress Fields 15 A. Experimental details 15 B. Simulated vacancy stresses 17 C. Continuum elastic theory 19 1. Linear elasticity 19 2. Geometric nonlinearity 20 3. Nonlinear elasticity 20 4. Vacancy interaction 21

IV. Dislocation Stress and Strain Fields 23 A. Experimental details 23 B. Simulated dislocation stresses 23 C. Continuum elastic theory 23 D. Strain ﬁelds 25 E. Elastic moduli 25

V. Polycrystal Stress Fields 27 A. Experimental details 27 B. Simulated polycrystal stresses 29 C. Virial stresses 30

References 31

2

2 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION

I. DERIVATION OF THE SALSA METHOD

A. Derivation

For a hard-sphere colloidal system, its bulk pairwise Brownian stress can be calculated by an integral over the three-dimensional pair correlation function g(r ) [1–4].

B σij = nkBTa rˆirˆjng(r )dS2 + nkBTδij (1) S2

Here, n is the number density of particles, kBT is the thermal energy, a is the particle radius, and i, j are the indices of the stress tensor. The second term is the ideal gas stress contribution arising from the kinetic energy. The oﬀ-diagonal components of the ﬁrst term, which usually dominate at high volume fractions, simply capture the anisotropy of g(r )

at contact surface S2. To determine the stresses at the particle-level, we write the pair correlation function, g(r ), as an ensemble average of delta functions.

k Ta N V σB = B rˆ rˆ δ(r r αβ)dS + nk Tδ ij Ω i j V N 2 − 2 B ij S2 α β =α 1 k Ta = B rˆ rˆ δ(r r αβ)dS + nk Tδ (2) N Ω i j − 2 B ij α S2 β =α where V , N, Ω are system volume, particle number, and particle volume, respectively. The bracket ... denotes an average over conﬁgurations and can be replaced with a time average in our system. In Eq. 2 we identify the outer sum as being an average over the particles in the sample, so we obtain an individual stress tensor for each,

k Ta σα = B rˆ rˆ δ(r r αβ)dS + nk Tδ ij Ωα i j − 2 B ij S2 β =α k Ta = B Ψ¯ α + nk Tδ (3) Ωα ij B ij

¯ α The elements of the sum Ψij can be identiﬁed as the fabric tensor linear density of particle α as the units work out to be [1/L]. This fabric tensor density directly reports the angular distribution of neighbors in contact with a particle while the magnitude of its trace ¯ α is related to the total number of neighbors. To calculate Ψij in simulation and experiment,

3

NATURE MATERIALS | www.nature.com/naturematerials 3 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

it is necessary to perform an average over a narrow interval ∆ 1

Ψ¯ α = rˆ rˆ δ(r r αβ)dS ij i j − 2 S2 β =α 1 a+∆ rˆ rˆ δ(r r αβ)dS dr ≈ ∆ i j − 2 S2 a β =α 1 = rˆαβrˆαβ (4) ∆ i j β ∆ ∈ where ∆ is the thickness of the measurement shell andr ˆαβ is the unit vector connecting the centers of particles α and β. Using this particular form, the SALSA formula reads

k T a σα = B rˆαβrˆαβ + nk Tδ ij Ωα ∆ i j B ij β ∆ ∈ k T a = B Ψα (∆) + nk Tδ (5) Ωα ∆ ij B ij α where Ψij can now be identiﬁed as the fabric tensor of particle α. In general, the shell thickness ∆ 1 should be small enough that the measurement result σα becomes indepen- ij dent of the particular choice of ∆. In the calibration section, we perform experiments and simulations to conﬁrm this independence. The details concerning the particle volume Ωα and converting the pointwise stresses to continuum ﬁelds are discussed in later sections. Finally, it is possible to extend our particle-level stress calculations to other ﬁnite poten- tials including the depletion force [5–7], paramagnetic [8] and electrostatic [9] interactions, and soft particles [10, 11]. While similar calculations have been performed at the bulk scale [8], extending our method to these systems would allow us to further investigate their heterogeneous elastic properties.

B. Local structural anisotropy tensor

The local structural anisotropy tensor reports the instantaneous arrangement of collid-

ing neighbors. The trace of this tensor,r ˆirˆi, is the total number of neighbors while the remaining terms capture the anisotropy of the collisions. As an illustration, we consider a two-dimensional case. Assuming one particle is at the origin and in contact with one other particle at an angle θ with respect to the x-axis then the fabric tensor can be written as

4 4 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION

2 rˆxrˆx rˆxrˆy cos θ sin θ cos θ rirj = = . 2 rˆyrˆx rˆyrˆy sin θ cos θ sin θ Here, the trace sin2 θ + cos2 θ is always 1 and a maximum shear is achieved at four locations,

θ = 45◦ and 135◦. These directions correspond to the maximal compression and ± ± 2 2 extension axes. For instance, if θ is 30◦, then the trace is (sin 30◦) + (cos 30◦) = 1, and the

shear component isx ˆyˆ =ˆyxˆ = (sin 30◦)(cos 30◦)=√3/4. Similarly, if θ is 90◦, while the

trace remains unity, the shear component becomesx ˆyˆ =ˆyxˆ = (sin 90◦)(cos 90◦)=0.

C. From pointwise functions to continuum ﬁelds

In the literature of molecular dynamics simulation, the virial 1 ∂V (r) r r sα = i j + mv v (6) ij 2 ∂r r i j β=α has been widely used to report stresses at the atomic level [12–14]. In particular, this quan- tity has been used to measure many interesting phenomena including the stress correlation length in liquid metals [13] and stress ﬂuctuations near grain boundaries [14]. While the sum

of the virials sij divided by system volume V yields the bulk stress of the system, there are multiple choices that can be made as to how to incorporate local volume variation and how to smooth the pointwise stress into a continuum ﬁeld. Similar to the Irving-Kirkwood-Noll procedure, which constructs continuum ﬁelds from the underlying discrete distribution with phase averaging, we perform a spatial average to obtain a macroscopic measurement at the cont particle-level [15]. The ﬁnal continuum stress ﬁeld σij (x ; t) is given by

cont pt σij (x ; t)= w(y x )σij (x ; t)d y (7) y − ∈R pt where w(r ) is a weighting kernel function, and σij (x ; t) is the pointwise function. Here, the weighting function w must be normalized so that the total energy is conserved during spatial averaging. We use a normalized Gaussian function that weights values closer to x more strongly than other points that are further away:

r2 3/2 3 2 − 2rw w(r)=π− rw− e (8)

5

NATURE MATERIALS | www.nature.com/naturematerials 5 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

(a) (b)(a) (c)(b) (d)(c)

FIG. 1: Spatially smoothed stress ﬁelds of a simulated polycrystal We plot the smoothed

stressed ﬁeld of a polycrystal as a function of ﬁlter size rw/2a at (a) 0.2 (b) 0.3 and (c) 1. For small

rw/2a, only the points containing particle centers with assigned stresses have nonzero values. As

the value of rw/2a increases, the stress ﬁeld becomes smoother and more continuous. Note that since the weighting Gaussian function is normalized, the overall stress of the system is the same for

all diﬀerent rw/2a. The color scale is adjusted for each sub ﬁgure to emphasize the stress variation

features. In all calculations, we use the value rw/2a = 1, where the features of individual particles are no longer distinguishable.

where r = r , and the ﬁlter size r is chosen to emphasize the length scale of the continuum w ﬁelds of interest [15]. Similar smoothing algorithms have been implemented in previous literature [16–19].

In our experiments and simulations, we set rw/2a = 1 so that we remove stress features on length scales smaller than a particle. The pointwise stress is constructed by ﬁrst assigning α α calculated particle virial, σijΩ to their corresponding grid boxes, then dividing their values by the box volume. This pointwise function shows singularities at particle centers and zero elsewhere. Finally, we smooth the ﬁeld using the Gaussian kernel, Eq. 8. We show the

spatial averaged continuum ﬁelds of a simulated polycrystal for three diﬀerent ﬁlter sizes rw in Fig. 1. In this spatial averaging procedure, the inﬂuence of local volume variation on the stress distribution is already incorporated. In particular, as the occupied volume of a particle increases, the stress is proportionally reduced due to the increased eﬀective averaging volume. Furthermore, the ﬁnal ﬁelds are nearly independent of the grid size and the mean stresses

6

6 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION

size = 1.0 (2a) size = 1.3 (2a) size = 2.0 (2a) size = 2.7 (2a) size = 4.0 (2a) (a) L (b) 2424 mPa size = 1.0 (2a) — current H size = 1.3 (2a) 2020 size = 2.0 (2a) size = 2.7 (2a)

Pressure (mPa) Pressure 16

Pressure 16 0 2 0 Distance2 (r/2a) Distance r 2a

FIG. 2: Spatially smoothed stress ﬁelds of a vacancy. (a)The values of smoothing length

scale rw from left to right are 1.0 2a, 1.3 2a, 2.0 2a, 2.7 2a and 4.0 2a, respectively. (b) The × × êH × L × × radial distribution of pressure for diﬀerent rw.

are constant at all values of rw.

To explore how the ﬁlter size rw aﬀects our ﬁnal SALSA stress ﬁelds, we show the ex-

perimental vacancy stress ﬁeld, σxy for ﬁve diﬀerent values of rw in Fig. 2(a). We ﬁnd that

the feature of the stress quadrupole [45] remains discernible up to rw =2.7(2a). Note in Fig. 2(a), while the quadrupole distribution theoretically diverges as 1/r3, it is cut oﬀ by the

lattice and smoothed over the distance rw, squelching the stress features near the vacancy core. Similarly in Fig. 2(b), we ﬁnd that the near ﬁeld of the pressure is strongly aﬀected by

the ﬁlter, but the long-range nonlinear pressure ring at rw = 1(2a) and 1.3(2a) match each other. Indeed, the long-range stresses from all defects have correspondingly slow variations,

and hence will be invariant to the choice of rw. The ﬁlter size choice is a balance – hiding

noise at lengths r

7

NATURE MATERIALS | www.nature.com/naturematerials 7 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

these terms, consider how smoothing changes a linear elastic free energy

= d3rS σ σ (9) F0 ijkl ij kl

where Sijkl is the elastic compliance tensor and σij is the stress tensor. If we smooth the

stress tensor using a Gaussian kernel of size rw this linear elastic theory changes to

3 3 3 k2r2 /2 ik r k 2r2 /2 ik r = d rd kd k S [σ (k)e− w e · ][σ (k )e− w e · ] F ijkl ij kl 3 k2r2 = d kS σ (k) σ ( k) e− w ijkl ij kl − S d3k (1 k2r2 ) σ (k) σ ( k) ≈ ijkl − w ij kl − = d3kS σ (k) σ ( k) d3kS k2r2 σ (k)σ ( k) ijkl ij kl − − ijkl w ij kl − = r2 d3kS (k σ (k))(k σ ( k)) F0 − w ijkl m ij m kl − What new terms must we add to to cancel the second term? Since each factor of F k introduces a gradient, we can check that a stress gradient term Sijkl∂m∂mσijσkl has the correct form.

3 3 3 3 ik r ik r Sijkl d r∂m∂m(σij σkl)=Sijkl ∂m∂m d rd kd k e− · σij(k) e− · σkl(k ) 3 3 3 ik r ik r = 2S d rd kd k k k e− · σ (k) e− · σ (k ) − ijkl m m ij kl = 2S d3kk k σ (k)σ ( k) − ijkl m m ij kl −

Indeed, the energy regularized by smoothing by rw is the original free energy plus a ﬁlter size-dependent term times a stress gradient energy:

2 rw 3 + S d r∂ ∂ (σ σ ) (10) F ≈F0 2 ijkl m m ij kl Similarly, nonlinear and other terms in the energy will produce regularization-dependent counter terms. We will now demonstrate that these gradient terms contribute less to the free energy than other nonlinear terms in the case of hard sphere crystals. Let us consider the long and short wavelength behavior of the ﬁrst nonlinear and gradient terms of the elastic free energy to see which dominates the behavior both close and far from a defect. For isotropic elasticity, the allowed terms that arise in the free energy density are

= C + D + E ∂ ∂ (11) F ijkl ij kl ijklmn ij kl mn ijklmn i j kl mn 8

8 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION

where the allowed elements of the elastic constant tensors C, D, and E are determined by the symmetries of the system being studied. In the case of isotropic materials, these tensors must be built using terms that are formed by δ and ∆ and , the Kronecker delta ij ijkl Dijklmn and the four and six index equivalents of the Kronecker delta. That is, the parts of the free energy may be written

= c + c FC 0 ii jj 1 ij ij = d + d + d FD 0 ii jj kk 1 ij ij kk 2 ij jk ki = e ∂ ∂ + e ∂ ∂ + FE 0 i i jj kk 1 i j ij kk ···

Which terms should we keep to describe the elastic ﬁelds? We consider their contributions in the case of the elastic ﬁeld of a vacancy defect – since the displacement ﬁeld for linear theory goes as u(r) ∆V/r2, the strain ﬁeld goes as ∆V/r3. The quadratic term ∼ ∼ 6 3 then has energy density which scales as r− , while the nonlinear cubic term ( ) scales as 9 1 1 3 3 8 r− and the gradient term as r− r− r− r− = r− . For short range behavior, the nonlinear contributions are nearly equal, with the cubic term contributing more for r 1. However, we also need to consider the magnitude and scaling of the coeﬃcients for each term. In the case of the cubic elastic constants, we know from the equation of state that the pressure 1 diverges at maximal packing as P (φ φ)− , implying that e.g. the bulk modulus diverges ∼ c − ∂P 2 as K = φ (φ φ)− [20]. If we write the scaling in terms of the two length scales in ∂φ ∼ c − the problem, the lattice constant a and the surface to surface distance ∆, we ﬁnd that the 2 9 2 8 cubic term in the free energy goes as (a/∆)− r− and the ﬁrst gradient term as a r− . In the case (a/∆) 1, we ﬁnd that the cubic terms dominates the gradient contributions. It is for this reason as well as the fact that gradient terms are not unique in our smoothing scheme that we only consider nonlinear elasticity without gradient terms.

II. CALIBRATION OF THE SALSA METHOD

To validate our SALSA measurements, it is crucial to calibrate the method and evaluate its performance and dependence on input parameters. We divide the calibration section into three parts: A) comparison with simulation stresses, B) contact criteria dependence, and C) force balance in a smoothed ﬁeld. We show that the SALSA method accurately captures the stress ﬁelds as calculated by Brownian dynamics very well. The stress ﬁeld

9

NATURE MATERIALS | www.nature.com/naturematerials 9 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

determined by using SALSA is not signiﬁcantly sensitive to the particle contact criteria e.g. the shell thickness ∆. Finally, we discuss a systematic residual force within the vacancy core in the continuum stress ﬁeld due to the smoothing process and compare the elastic ﬁelds to similarly smoothed continuum calculations.

A. Calibration: SALSA versus actual stress

To evaluate how well SALSA is able to report the correct stress ﬁeld of a complex sys- tem, we use Brownian dynamics (BD) to generate a vacancy in a simulated crystal, whose orientation is matched to that found in our experiments. We use SALSA to determine all six independent stress components and compare their values with the BD stress calculation using the same set of position data (see Fig. 3). The continuum stress ﬁeld from BD is

constructed by spatially averaging pointwise virials Fixj. We see that the BD and SALSA stresses exhibit a good match. We also ﬁnd that SALSA stresses become more quantitatively similar to the actual stress ﬁelds as a longer time-average is performed (not shown).

σxx σyy σzz σxy σxz σyz SALSA Virial stress Virial

FIG. 3: SALSA and actual stresses comparison. Stresses determined through the SALSA method (top row) are compared with the stresses directly calculated in simulation (bottom row) using the same dataset.

B. Calibration: Contact criteria dependence

There is another parameter in the SALSA method, which is the shell thickness ∆ used to identify particles in contact. This shell thickness directly determines the number of particles

10

10 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION L g

D 5 H

P 2 Lê

D 1 H

P 0.5 0.2 Experiment 0.1 Simulation 0.05 Δg 2a Pressure 0.02 0.01 0.02 0.05 0.1 0.2 D 2a

FIG. 4: SALSA pressure versus ∆ in experiment and simulation. Pressure measured using êH L diﬀerent shell thickness ∆ is plotted as a function of ∆. The pressures values P(∆) are normalized

by P(∆g) where ∆g +2a is the position of the g(r) ﬁrst peak, which is denoted by the gray line. The vacancy experimental data (red curve) shows that SALSA method generates quantitatively consistent results in a wide range of shell thickness 0.03(2a) ∆ 0.15(2a) (shaded area). The ≤ ≤ corresponding length scale of this thickness range is 40 nm ∆ 230 nm. The simulation data ≤ ≤ (blue curve) demonstrate an even wider pressure plateau that extends beyond ∆ 10 4(2a). The ∼ − diverging trend of the experimental pressure at small ∆ occurs due to slight particle overlaps arising from featuring uncertainties.

that are included in the stress calculation, larger ∆ allowing for shorter time averages. However, at large ∆, the radial distribution of particles g(r) will vary through out the thickness of the shell, leading to systematic errors in stress. We test for the optimum by calculating the pressure of a system versus ∆/2a. Fig. 4 shows the SALSA pressure

P (∆)/P (∆g) versus ∆/2a for both experimental and simulation data. Here, ∆g/2a (gray line in Fig. 4) is the cutoﬀ thickness used throughout our analysis of the experiments, where

2a +∆g roughly coincides with the ﬁrst peak of g(r). We ﬁnd that the measured pressure has negligible dependence on ∆/2a for ∆/2a 0.12. In the experiment the normalized ≤ pressure deviates from 1 when ∆ is smaller than 3% of the particle size, corresponding ∼ to 1/4 of a pixel ( 35 nm). This trend arises due to particle overlaps from featuring ≈ ∼ uncertainties. Overall, as shown in Fig. 4, both the experimental and simulation results indicate an insigniﬁcant correlation between the SALSA pressure and shell thickness ∆ in

11

NATURE MATERIALS | www.nature.com/naturematerials 11 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

the range of 35 nm ∆ 230 nm (yellow shaded area). ≤ ≤

Pressure σxy (a) L r H g

1.2 1.4 Distance mm (b)

L H L r H g

1.2 1.4 Distance mm (c)

L H L r H g

1.2 1.4 Distance mm (d) H L L r H g

1.2 1.4 Distance mm

H L FIG. 5: Pressure and σxy ﬁelds for diﬀerent ∆ Pressure (middle row) and shear stress σxy (right row) distributions for four diﬀerent values of shell thicknesses. (c) The contact criteria used throughout our experiments. The pair correlation functions g(r) (left row) are plotted to illustrate the diﬀerences between the shell thickness ∆ choices (orange lines).

Finally, we also investigate how the shell thickness ∆ aﬀects the spatial distribution of

stresses. We show the experimental pressure and σxy ﬁelds near a vacancy for four diﬀerent ∆ in Fig. 5. Again, we ﬁnd that the stress ﬁelds for all ∆ demonstrate qualitatively similar

trends, where the pressure exhibits an enhancement surrounding the defect core and σxy shows a quadrupole distribution. This weak ∆ dependence is consistent with the previous experimental studies [21, 22] where the authors have found that diﬀerent contact criterion consistently generate similar bulk Brownian stresses. Here, we provide a similar calibration but at the particle level. As shown in Fig. 5, it is remarkable that SALSA is able to produce consistent results with a wide range of shell thickness 35 nm ∆ 150 nm. This wide ≤ ≤

12 12 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION

Simulation (a) ∂σjx/∂x ∂σjy/∂y ∂σjz/∂z Total force j=x

∂σxx/∂x ∂σxy/∂y ∂σxz/∂z Fx j=y

∂σyx/∂x ∂σyy/∂y ∂σyz/∂z Fy j=z

∂σzx/∂x ∂σzy/∂y ∂σzz/∂z Fz Continuum model (b) ∂σjx/∂x ∂σjy/∂y ∂σjz/∂z Total force j=x

∂σxx/∂x ∂σxy/∂y ∂σxz/∂z Fx j=y

∂σyx/∂x ∂σyy/∂y ∂σyz/∂z Fy j=z

∂σzx/∂x ∂σzy/∂y ∂σzz/∂z Fz

FIG. 6: Force balance of vacancy. The right-most frames show the divergence of the stress ﬁelds from simulation (a) and continuum theory (b). In the group of nine panels in each of these subﬁgures, we show the components of the divergence of the stress. Summing along each row, we ﬁnd the total force as the sum of the gradients. Both the BD simulation and continuum elastic ﬁelds show systematic force dipoles in their center indicating that the small residual forces are produced not from the SALSA method but from the choices made in creating a continuum ﬁeld.

window of ∆ choice promises robust stress measurements in the typical colloidal experiments with 3D imaging, where the particle positions can be precisely determined with a sub-pixel resolution ( 50 nm) using standard featuring algorithms. ≤

13

NATURE MATERIALS | www.nature.com/naturematerials 13 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

C. Calibration: Mechanical equilibrium of a smoothed ﬁeld

In principal, it is possible to further determine the continuous force ﬁeld by calculating the divergence of the smoothed stress distribution. In our experiments, where all the stud- ied regions are stationary, the calculated force ﬁeld should be zero implying a mechanical equilibrium. It has recently been shown that this mechanical equilibrium of the microscopic stress closely depends on the details of the stress deﬁnition at particle-level [23]; it is im- portant to check it for SALSA. To investigate this issue, we calculate the divergences of the vacancy SALSA stresses in simulation (Fig. 6 (a)). We ﬁnd that the force ﬁelds are consistent with zero everywhere except the region of the defect core, where the force shows a dipole distribution in all components. Since there is no particle in the region that violates mechanical equilibrium, it is unclear whether this force imbalance leads to a particle drift or not. Nevertheless, to conﬁrm that this is only a result of the smoothing procedure, we perform a similar analysis on calculated continuum elastic ﬁelds. In doing so, we mimic the SALSA measurements by introducing a pressure hole in the center, and smooth the stress ﬁelds with the same kernel used in the simulation. As shown in Fig. 6 (b), the force ﬁelds from continuum theory also display force dipoles consistent with SALSA and BD stress ﬁelds. This consistency clearly indicates that the force imbalance mostly arises from the pressure drop and smoothing algorithm rather than the SALSA calculation. To further characterize the magnitude of the force imbalance, we perform a similar me- chanical equilibrium calibration in a simulated polycrystal. In particular, we construct a three dimensional box enclosing a grain boundary. Then we determine the net force acting on this box by calculating the tractions from stresses. We ﬁnd that the forces correspond to the shear and normal tractions approximately cancel each other, indicating a good me- chanical equilibrium. The residual force can then be related to a drift arising from this force imbalance given that the system is over-damped. Finally, we ﬁnd that the drift, which is independent of the box size, is less than 5% of the particle diameter over the entire simulation.

14

14 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION

III. VACANCY STRESS FIELDS

A. Experimental details

We create a colloidal crystal consisting of 1.3 µm diameter silica particles via sedimenta- tion in a sealed sample cell. The particles are suspended in a water-glycerol mixture with a refractive index matching the silica particles. This matched refractive index allows us to acquire confocal images of the sample. Vacancy defects form spontaneously during sedi- mentation (along with stacking faults and grain boundaries), and are imaged directly using a high-speed confocal microscope. In the measurements, we select isolated vacancies that contain no other defects within ﬁve lattice spacings in the plane or in either of the adjacent layers perpendicular to the plane. Since the system is thermal, it is important to perform a time average to correctly de- termine the equilibrium stress ﬁeld. Therefore, we record, analyze, and average the stress ﬁelds over 60 snapshots (20 seconds). We further average the stress ﬁeld over 20 vacancies to reduce the eﬀects of polydispersity and the local vacancy environment. In Fig. 7, we show the confocal images of all measured vacancies in the experiment (the horizontal slices of full 3D confocal image stacks) to illustrate the vacancy morphology. As shown in Fig. 7, the independent vacancies have random orientations with respect to the microscope and must be aligned before averaging. With all images aligned in the same orientation, we then calculate the stress ﬁeld of each sample and average over 20 seconds. This time interval is suﬃciently long for the colloids to explore the local phase space as the time required to diﬀuse one particle separation (100 nm) in the absence of obstructing neighbors is about 0.35 s. Finally, we average the per-vacancy stress ﬁeld over all 20 samples. Since SALSA solely relies on the particle positions to determine the stress ﬁeld, the cor- rectness of ﬁnal measurements directly depends on the accuracy of particle featuring and noise in the experiment. We employ both time and sample averages to remove noise and improve such measurement accuracies. Uncorrelated noise such as the current noise in the electronics, can be eﬀectively reduced by using a time average. On the other hand, there is correlated noise that result in a persistent featuring bias in time, including spherical aberration in the optics [24–26], the microscope point-spread-function [27–29], and particle polydispersity [30]. In the vacancy experiment, we minimize the eﬀects of spherical aber-

15

NATURE MATERIALS | www.nature.com/naturematerials 15 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

FIG. 7: Confocal images of 20 isolated vacancies.

ration and point-spread-function by index-matching the sample within 0.1% and conﬁning the imaging ﬁeld to a few particles away from the coverslip. Polydispersity also aﬀects our ability to determine which particles are in contact. For instance, when two larger particles are touching, the SALSA method may identify them as not in contact because their center- to-center distance is larger than 2 a +∆, the mean distance between particles plus the shell thickness. The polydispersity ( 35 nm for our silica colloids) is about 30% of the shell ≈ thickness ∆ = 106 nm used in our experiment. In the vacancy experiment, by averaging the stress ﬁeld over 20 diﬀerent samples, the collision uncertainty due to polydispersity is further reduced by a factor of √20 = 4.5. Furthermore, we ﬁnd that the polydispersity has diﬀerent eﬀects on the pressure and

shear stress measurements. We show two representative stress components σxx and σxy, ﬁrst time averaged, Fig. 8 (a) and (b), and then with an additional sample average, Fig. 8 (c) and (d). We ﬁnd that the pressure does not fully capture the enhanced stress ring around the vacancy defect if only a time average is applied. However, the shear component of the same time-averaged data already shows a clear quadrupole structure that is very similar to the one with additional sample averaging. This ﬁnding implies that while the pressure measurement may rely on a more precise identiﬁcation of touching particles, the shear measurement is relatively robust and insensitive to the noise. In contrast to the normal

16

16 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION

(a) (b)

time-average only

6.4 σχχ σχy 2 5.8 (c) (d) -2 (10-2Pa) (10-3Pa)

with sample-average

σχχ σχy

FIG. 8: Eﬀects of sample average. Comparison of time average and sample average on a

normal component σxx (a,c) and shear component σxy (b,d). We see that sample average improves the measurement of the normal component more than the shear components due to the eﬀects of polydispersity.

stresses that are strongly associated with the collision (touching) probability of surrounding particles, the shear components are more related to the angular anisotropy of the neighboring particle conﬁgurations. Finally, it is also possible to avoid the eﬀects of polydispersity by determining the individual particle size and taking the size variation into account [31].

B. Simulated vacancy stresses

We conﬁrm the experimental ﬁndings by simulating the stress of a vacancy in a colloidal crystal using nearly hard-sphere Brownian dynamics. Here, we numerically simulate the Langevin dynamics of N particles interacting through a very sharp radial potential V (r). We do so using cell neighbor lists calculated on an NVIDIA GPU integrating with the velocity Verlet algorithm. The virials of each particle, calculated through Eq. 6, are used to compare directly to the stresses calculated with the SALSA method. Based on previous literature [22], we have tried several interparticle potentials including the Yukawa potential, pure power law, and smoothed power law. Here we use the smoothed

17

NATURE MATERIALS | www.nature.com/naturematerials 17 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

power law to ensure continuity in derivatives:

r 2 r 24 V (r)= 1 0 (12) E r0 − r To simulate the vacancy, we begin with a periodic cell of a fcc crystal with the same phys- ical parameters as the experimental setup. We create a periodic cell containing 214 = 16384 3 particles at a packing fraction of φ =0.59, temperature T = 300 kBT and viscosity η = 10 . We remove the center particle and simulate for 2500 snapshots where each snapshot is sep- arated by t = 10τ diﬀusion times. The stress of these particle conﬁgurations is calculated using both the simulation virial and SALSA and averaged over the entire simulation time. A direct comparison of these stress ﬁelds can be found in Fig. 3. We do ﬁnd some quantitative diﬀerences between the experiment and simulation. For example, the pressure of the simu- lated vacancy is plotted as a function of distance from the defect core in Fig. 9. While the morphology in each individual stress component is very close to that seen in experiments, we do not ﬁnd as strong of a pressure enhancement around the simulated vacancy. This softening is most likely due to the softened core of the potential we use. Overall, however, all the qualitative features are reproduced in each of experiment, simulation, and theory.

(a) (b) L L 24.6 Simulation 24 mPa mPa H H 24.4 20 Experiment Theory Simulation Pressure

Pressure 16 24.2 0 2 4 0 2 4 Distance r 2a Distance r 2a

FIG. 9: Vacancy pressure distribution Comparison of experimental (blue dots in (a)), theoret- ical (red line in (a)), and simulation (green line in (b)) pressure. Despite its relatively insigniﬁcant êH L êH L feature, the simulated vacancy pressure also exhibits a pressure enhancement at r 4a. All indi- ∼ vidual stress components in experiment, theory, and simulation show qualitatively similar results.

18

18 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION

C. Continuum elastic theory

1. Linear elasticity

To further measure the performance of SALSA, we also compare the stress ﬁelds calcu- lated in simulation and experiment to the corresponding continuum elastic theory. In linear isotropic elastic theory, a vacancy’s displacement ﬁeld can be described by a radial function 2 determined entirely by the local volume change ui(r)=∆V/r rˆi. This can be seen by looking at the elastic free energy which can be written

1 = K2 + µ( 1/3 δ )2 (13) Flinear 2 ii ij − ij ll

where K is the bulk modulus, µ is the shear modulus and ij the strain tensor, the sym-

metrized Jacobian of the displacement ﬁeld u, ij =1/2(∂iuj + ∂jui). Since the material

is isotropic, we make u a radial function such that ui(r )=u(r)ˆri. We then minimize the free energy with respect to this displacement ﬁeld through the Euler-Langrange equations ∂F ∂ ∂F 2 = 0, giving a diﬀerential equation for the displacement r u +2ru 2u =0 ∂ui − ∂xi ∂∂ui − whose solution is given by ∆V P u(r)= + ∞ r (14) 4πr2 3K Here, ∆V is the local volume change, P is the pressure at long length scales due to boundary ∞ conditions and K is again the bulk modulus. This displacement ﬁeld leads to a strain and stress ﬁeld in linear elasticity that has the form

1 = (∂ u + ∂ u ) ij 2 i j j i u rirj rirj = δ + u r ij − r2 r2 σ = K δ +2µ( 1/3δ ) ij ll ij ij − ij kk u u 1 rirj = K 2 + u δ +2µ u δ r ij r − 3 ij − r2 Using this stress ﬁeld, we ﬁnd the pressure ﬁeld is a constant

u P = σii/3=K 2 + u = P (15) r ∞

19

NATURE MATERIALS | www.nature.com/naturematerials 19 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

2. Geometric nonlinearity

However, both the simulation and experimental data show a pressure ring that suggests we need to move to higher order elasticity to accurately describe the stress ﬁeld of the colloidal vacancy. The ﬁrst natural attempt to capture this ring can be done by including the geometric nonlinearity (also known as ﬁnite strain), an extra term in the strain ﬁeld that makes it rotationally invariant but is higher order in displacement. Doing so, we ﬁnd that

1 = (∂ u + ∂ u + ∂ u ∂ u ) ij 2 i j j i i k j k 2 u rirj rirj 1 u rirj 2 rirj = δ + u + δ + u r ij − r2 r2 2 r ij − r2 r2 rirj rirj = U¯ δ + U¯ ij − r2 r2 2 2 where we can deﬁne U¯ = u/r +1/2(u/r) and U¯ = u +1/2u . We then calculate the stress which is linear in the strain, arriving at the same answer as previously, except with these variables substituted. Lastly, we ﬁnd the diﬀerential equation for the radial displacement ﬁeld via the Euler-Lagrange equations, yielding a long nonlinear ODE, which we omit for brevity. Fitting the experimental data using this form yields a small pressure enhancement which cannot be tuned to quantitatively match the experimental data without resorting to unphysical values for the bulk and shear modulus.

3. Nonlinear elasticity

Motivated by arguments made in Section II, we next calculate the stress ﬁeld incorpo- rating the leading terms in nonlinear isotropic elastic theory. In particular, we modify the free energy such that

α β γ = + + + (16) F Flinear 3 ii jj kk 6 ij jk ki 4 ii jk jk

We insert the deﬁnition of ﬁnite strain into the new free energy to arrive at another

20

20 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION

diﬀerential equation for the displacement ﬁeld as a function u(r).

5 5 r (24r(λ +2µ)u (r)+6(α + β + γ)u (r)

3 +4u (r) (2(8α + 3(4β +2γ + λ +2µ)) + 15r(α + β + γ)u (r))

2 +4u (r) (8α + 6(2β + γ +4λ +6µ)+9ru (r)(2α +2β +2γ + λ +2µ))

+ 24u (r)(2(λ +2µ)+ru (r)(α + β + γ +3λ +6µ))

4 4 +3u (r) (2(6α +8β +5γ)+5r(α + β + γ)u (r))) + 2r u(r)(8(r(α + 3(β + λ))u (r)

4 3 2 3(λ +2µ)) + 3(α +3β)u (r) + 12(α +3β)u (r) +4u (r) (5α + 3(6β + λ)+3r(α +3β)u (r)) − 3 2 +8u (r)(α + 3(β + λ)+3r(α +3β)u (r))) + 4r u(r) (2(r(2α +9β +3λ)u (r)

2 3(2α +4β + γ +6λ +6µ))+3u (r) (α +6β + r(α +3β)u (r))+6r(α +3β)u (r)u (r)) − 2 3 2 +4r u(r) (2( 13α 6(5β + γ + λ + µ)+r(α +6β)u (r))+(α +6β)u (r) 2(α +6β)u (r)) − − − 4 5 +2ru(r) ( 32α 72β 15γ + r(α +6β)u (r) 2(α +6β)u (r)) 6u(r) (2α +4β + γ)=0 − − − − −

We use this nonlinear ODE to ﬁt the pressure proﬁle found in the experimental data using only the purely compressional third-order elastic constant α =3.6 Pa, leaving β = γ = 0. In this same ﬁt, we set the other elastic constants K =0.093 Pa and µ =0.092 Pa based on studies of hard sphere elastic constants [32]. We also set the volume change ∆V = 0.083 to − be the same as the experimental value. In this ﬁt, we are able to reproduce the experimental

pressure ring with one third-order elastic constant and one initial condition (u far from the vacancy). The value of α we ﬁnd from our ﬁt of the pressure ring is consistent with the variation of bulk modulus with packing fraction as calculated by hard sphere simulations. We can directly compare these values using the equation of state. Given the pressure of a hard sphere system as a function of packing fraction, P (φ), we can expand the elastic constants 1 2 as K(φ )+K (φ )(φ φ )+ K (φ )(φ φ ) + giving α = K (φ )=∂ (φ∂ P ) . 0 0 − 0 2 0 − 0 ··· 0 φ φ |φ0 Using the functional form for P (φ) we get that α(0.59) 3.0 Pa in agreement with our ﬁt ≈ α =3.6 to experimental stresses using nonlinear elasticity.

4. Vacancy interaction

The overall sign of the interaction between vacancies must be negative as vacancies are in general attracted to areas of higher pressure just as interstitials are attracted to areas of

21

NATURE MATERIALS | www.nature.com/naturematerials 21 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

lower relative pressure. In the case of two vacancies, the local increase in pressure around one vacancy acts as a higher pressure region for the second, causing them to mutually attract. Physically speaking, the collapse of particles towards the core of one vacancy causes particles to collide more frequently which is relieved by the negative volume change given by the second vacancy. The above argument gives the dominant nonlinear term (the linear ﬁeld of one vacancy coupling to the nonlinear pressure around another). Higher order eﬀects can be repulsive but are smaller than this leading order term. Speciﬁcally, to calculate the attraction or repulsion of vacancies, we look at the elastic free energy, which strictly speaking is entirely entropic. In this treatment, we will be calling all entropic contributions aside from the conﬁgurational entropy the elastic energy E , giving us a free energy density = E TS . To elastic F elastic − conf ﬁrst order, the elastic energy density is Eelastic = σijij where σ is stress and is strain. We consider the perturbative view of the elastic free energy in the case of the interaction

of two vacancies A and B, which can be expanded into three primary terms, Eelastic = A,L B,L A,N B,L A,N B,N σij ij +2σij ij + σij ij where L indicates a linear contribution and N indications a nonlinear one. In isotropic linear elastic theory, vacancies do not interact making the ﬁrst term independent of vacancy separation and leaving us with the second and third terms of the expansion. The second term is the linear part vacancy B’s quadrupole strain ﬁeld sitting in the nonlinear (pressure bump) stress ﬁeld of vacancy A. In this simple case, we ext B know that the energy can be given by the vacancy quadrupole E = σij Qij, where the B B ext A,N strain quadrupole for a vacancy is diagonal Qij =∆V δij and σ = σ is an external ext B stress ﬁeld given by vacancy A. Therefore, the energy can be written E = σii ∆V = σA,N∆V B = P A,N∆V B. Since ∆V 0 for vacancy defects, this term is negative, leading to ii ≤ an overall attraction, consistent with previous literature [33–36]. This calculation will have higher-order corrections due to the nonlinear elastic overlap of the nonlinear pressure rings P A,NP B,N as well as nonlinear corrections to the pressure bump itself due to the presence ∝ of a second vacancy, but the qualitative behavior remains unchanged.

22

22 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION

IV. DISLOCATION STRESS AND STRAIN FIELDS

A. Experimental details

The dislocation is produced by templating the [100] axis on a glass coverslip at a registry 1.5% larger than the equilibrium lattice constant [37]. Particles are sedimented onto the substrate forming a single face-centered cubic crystal. As the crystal thickness reaches about 31 µm, a signiﬁcant number of dislocations spontaneously nucleate and grow. We then image the three dimensional microstructure of an isolated dislocation using a confocal microscope. A schematic of these dislocations is found in the main text.

B. Simulated dislocation stresses

To closely simulate the particular dislocation studied in the experiment, we import the experimentally measured particle positions into the Brownian dynamics simulation. Prior to recording the stress, we relax the system to remove overlaps using a soft Hertzian potential and a large damping factor to ensure very little rearrangement. We then freeze the border particles as labeled in red in Fig. 10 to ensure that the topologically constrained dislocation does not migrate. After performing a time average, we ﬁnd that the calculated stress ﬁeld, both through virial calculation and SALSA method, are in excellent agreement with the experiment, providing a conﬁrmation to the SALSA measurements. Importantly, since this simulation procedure only requires a single snapshot of data for the initial condition, this technique can be particularly useful in determining stresses in the experimental cases where time average is challenging. For instance, it is diﬃcult to perform a time average in a system where the ﬂuorescent dye photobleaches signiﬁcantly or the dynamic time-scale is comparable to the time between acquisition of successive image stacks.

C. Continuum elastic theory

To compare against isotropic linear elasticity, we again calculate the stress ﬁeld of the dislocation. The stress ﬁeld of a dislocation in coordinates where z is along the dislocation

23

NATURE MATERIALS | www.nature.com/naturematerials 23 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

Compressive strain Shear strain γxz 0.10 0.10 Frozen 0.2 0.1 particles 0.2 0.2 0.2 0.1 0.1 0.1 0.1 0.10.05 0.1 0.1 0.05 High 0.05 0.05 0.05 0.05 0 z 00 0 0 0 z-height x 2 μm 0 0 −0.1 −-0.050.1 −0.1 -0.05 0 0 −0.1 Low FIG. 11: Strain ﬁelds of a dislocation. Experimental measurements of strain using the tech- Dislocation line nique of Falk et al. [40] showing both compressive (left) and shear (right) strain distributions near a dislocation defect. The approximate location of the dislocation core is labeled with a ( ). Notice x ⊥ y z that while the trend is very similar to that of the dislocation stress ﬁeld (as in linear elasticity), there is a stronger divergence towards the core which is highlighted in the main text in Fig. 3.

experiment and simulation. Doing so, we ﬁnd an excellent agreement with the other methods FIG. 10: Frozen particle border (dislocation). A screen-shot of our Brownian dynamics as shown in the main text Fig 3. simulation of the experimental fcc crystal. In shades of gray are active hard sphere particles while

in red are the frozen boundary particles. Luminance in this picture roughly indicates the position D. Strain ﬁelds in the z direction with only a thin slice of the entire simulation shown and darker colors indicating being deeper into the page. The dislocation line is visible 1/3 from the bottom of the image running To investigate the relation between stress and strain, we determine the strain ﬁeld near the dislocation. Following a previously developed algorithm [40], we measure the particle-level left to right as indicated by the discontinuity in particle shade between adjacent rows. strain by quantifying the local aﬃne deformation of individual particles. The compressive

line, is given by [38] and shear strain (γxz) ﬁelds are shown in Fig. 11. We ﬁnd that the strain ﬁelds show 3x2 + y2 qualitatively similar features found in the stress distributions. However, as illustrated in σxx = y − (x2 + y2)2 Fig. 3(c) of the main paper, the stress-strain curve deviates from linearity near defects x2 y2 σ = y − where strains are large. yy (x2 + y2)2 x2 y2 σxy = x − (x2 + y2)2 E. Elastic moduli

σzz = ν(σxx + σyy) Using the strain measurement, we analyze other experimentally accessible cubic moduli Using the method known as Dislocation Extraction Algorithm (DXA), we extract the line as done in the main manuscript. To that end, we compute the compressive C33 and shear C13 dislocation for our partial dislocation [39]. We rotate and translate the theoretical stress modulus proﬁles and discuss their behaviors below. We focus on the moduli associated with ﬁeld for a single dislocation, integrating along the length of the dislocation as done in the the strain component γzz, which shows a larger response than γxx and γyy in our experiment.

24 25

24 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION

Compressive strain Shear strain γxz 0.10 0.10 0.2 0.2 0.2 0.2 0.1 0.1 0.1 0.1 0.1 0.05 0.05 0.1 0.1 0.1 0.05 0.05 0.05 0.05 0 z 00 0 0 0 x −0.1 2 μm−0.1 0 0 0 −0.1 -0.05 −0.1 -0.05 0

FIG. 11: Strain ﬁelds of a dislocation. Experimental measurements of strain using the tech- nique of Falk et al. [40] showing both compressive (left) and shear (right) strain distributions near a dislocation defect. The approximate location of the dislocation core is labeled with a ( ). Notice ⊥ that while the trend is very similar to that of the dislocation stress ﬁeld (as in linear elasticity), there is a stronger divergence towards the core which is highlighted in the main text in Fig. 3.

experiment and simulation. Doing so, we ﬁnd an excellent agreement with the other methods as shown in the main text Fig 3.

D. Strain ﬁelds

To investigate the relation between stress and strain, we determine the strain ﬁeld near the dislocation. Following a previously developed algorithm [40], we measure the particle-level strain by quantifying the local aﬃne deformation of individual particles. The compressive

and shear strain (γxz) ﬁelds are shown in Fig. 11. We ﬁnd that the strain ﬁelds show qualitatively similar features found in the stress distributions. However, as illustrated in Fig. 3(c) of the main paper, the stress-strain curve deviates from linearity near defects where strains are large.

E. Elastic moduli

Using the strain measurement, we analyze other experimentally accessible cubic moduli

as done in the main manuscript. To that end, we compute the compressive C33 and shear C13 modulus proﬁles and discuss their behaviors below. We focus on the moduli associated with

the strain component γzz, which shows a larger response than γxx and γyy in our experiment.

25

NATURE MATERIALS | www.nature.com/naturematerials 25 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

For this analysis we rotate our stress and strain tensors so that the x and y axes align with the (100) and (010) axes of the cubic system. In this frame, the moduli for an cubic crystal

have the following symmetries: C33 = C22 = C11, and C23 = C13 = C12. To compute the compressive modulus near the dislocation core, we ﬁrst determine the

compressive stress σzz and strain γzz. Here, we determine the uniform background strain (due to the overall pressure arising from conﬁnement and gravity) by matching the measured modulus to the corresponding theoretical value [41]. We then perform the same analysis used

in the shear modulus calculation, and plot the compressive modulus C33 as a function of position r/2a in Fig. 12(a). The region of the dislocation core is at r/2a 5.5 (gray shade). ≈ We ﬁnd that C33 is higher on the side with an additional half plane of particles. Similarly,

we also observe a reduction in C33 on the other side due to the missing half plane of particles.

We also ﬁnd that the trend of the shear modulus C23 is similar to the compressive modulus

C33 (Fig. 12(b)), which shows an enhancement on the left side and a reduction on the right. The moduli we report are only calculated along a line perpendicular to the glide plane of the dislocation. The other two natural directions along the glide plane are excluded due to experimental limitations. Along the burgers vector we are limited by the noise in the stress and strain ﬁelds. Since the modulus is the ratio of the two, zeros remain problematic, similar to issues in deconvolution, and a new method of inference must be applied to the moduli in these regions. Along the dislocation line, we have already collapsed the data by averaging the stress and strain ﬁelds in this direction in order to reduce noise in the x-z plane. This averaging makes it infeasible to calculate the modulus variation in this direction. Due to symmetry, this direction should display a constant modulus. In the future, with a full time series of dislocation images, we can begin to look at the modulus variation near kinks and jogs along the dislocation line.

26

26 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION

(a) (b) L 0.14 L 0.14 Pa Theoretical Pa H Enhancement H value 0.12 33 23 C 0.12 C 0.1 0.08 0.1 Reduction 0.06 Modulus Modulus 1 3 5 7 9 1 3 5 7 9 Position r 2a Position r 2a

FIG. 12: Proﬁle of the cubic moduli C and C . (a) Compressive modulus C versus position êH 33L 23 êH 33L perpendicular to the glide plane of the dislocation. (b) Shear modulus C23 measured along the same direction. Both moduli are calculated using the protocol described in the main manuscript.

V. POLYCRYSTAL STRESS FIELDS

A. Experimental details

We show a confocal image of the polycrystal we use in our experimental analysis in Fig. 13(a). The shown ﬁeld of view is the same as the one of the stress ﬁeld reported in the main manuscript. We show only a slice in the x-y plane of a complete 3D image stack. The z-interval between adjacent scan slices is 0.135 µm 0.1 times the particle diameter. By ∼ matching the refractive indices of the water-glycerol mixture and silica particles, we minimize eﬀects from the point spread function and z-axis spherical aberration, thus optimizing the image quality. We show the featured particle position with green circles in Fig. 13 (a). The data are visually overlaid to ensure there are no missing or repeated features. To investigate the featuring accuracy, we plot the 1D g(r) of the suspension in Fig. 13(b). As indicated by the sharpness of the ﬁrst peak of g(r), limiting our ﬁeld of view to the ﬁrst ten layers from the coverslip (in the optical z direction) enables us to accurately feature the particle positions. The spread of this peak arises from three contributions: featuring errors, polydispersity, and the thermal ﬂuctuation of the equilibrium separation between particles. The location of the peak is primarily inﬂuenced by particle featuring errors and the packing fraction of the sample. While the polydispersity of this sample is σ2 5% a = 50 nm, this a ∼ variation in size will not shift the peak of g(r) from the mean particle diameter (Fig. 13) unless there are spatial correlations of particle size. Therefore, at most, the averaging

27

NATURE MATERIALS | www.nature.com/naturematerials 27 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

(a) (b) (c) 6 8 6 L r H g

L 4 r H 4 g 2 0 1.2 1.3 1.4 2 Distance r mm

0 H L 0.0 0.5 1.0 1.5 2.0 Distance r mm

FIG. 13: Colloidal polycrystal sample. (a) A representative slice of a 3D confocal image stack. H L Green circles illustrate the featured particle positions. This overlaid image shows that all particle positions are correctly identiﬁed without any missing particles. (b) The pair correlation function g(r) calculated using featured particle positions. In the inset we show that the amount of particle overlap (yellow region) is negligible. (c) A SEM micrograph of two particles showing how the true particle size was determined in the sample.

featuring errors should correspond to this peak shift of 50 nm. Furthermore, we show a SEM micrograph to illustrate the roundness of the colloidal particles and the smoothness of their surfaces, see Fig. 13(c). As shown in the SEM image, the surface roughness is less than the SEM resolution 5 nm. We also use the SEM image ∼ to measure the polydispersity of the silica colloids. We ﬁnd that the polydispersity of the sample is less than 3% of the particle size, consistent with the speciﬁcation provided by the manufacturer. In the stress measurement of the polycrystal, we average the calculated stress ﬁeld over 50 stacks of images. The structure of the polycrystal remains unchanged within the acqui- sition time ( 30 s). While we expect to observe short-time stress ﬂuctuations arising from ∼ particle Brownian motion within the acquisition time, we do not ﬁnd any signiﬁcant stress ﬂuctuations on longer time scales.

28

28 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION

FIG. 14: Frozen particle border (polycrystal). A screen-shot of our Brownian dynamics simulation of the experimental polycrystal. In shades of gray are active hard sphere particles while in red are the frozen boundary particles. Luminance in this picture roughly indicates the position in the z direction with only a thin slice of the entire simulation shown.

B. Simulated polycrystal stresses

As with the dislocation stresses, we veriﬁed that the experimental stresses are accurate using a simulation-experiment hybrid. Again we use the experimentally featured particle positions as initial conditions for our hard sphere Brownian dynamics simulation. For each experimental snapshot, we remove overlaps and freeze boundary particles as before, then evolve the system, measuring stresses using both the true virial measurements as well as SALSA. By averaging over the various snapshots, we arrive at a stress ﬁeld very similar to that found by the experimental SALSA calculation.

29

NATURE MATERIALS | www.nature.com/naturematerials 29 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

Pressure σxy (fabric) (fabric)

FIG. 15: Per-particle virials The experimental polycrystal with particles colored by the mag- nitude of the fabric tensor (directly proportional to particle virial). While we see large scale correlations of fabric tensor trace with grain interiors and variation of oﬀ-diagonal components between grains, the magnitude of variation is much smaller than that found in previous numerical studies of stress distributions in strained polycrystals [14]

C. Virial stresses

In simulation literature, the atomic-level stress has been referred to as the virial of an individual atom either normalized or un-normalized by the system volume [14, 42–44]. Here,

the virial Fixj can be considered to be a stress that does not account for the local variation of atomic (particle) free volume. To compare our experimental results with the previous simulation ﬁndings (which do not correct for local particle density ﬂuctuations), we plot (Fig. 15) the un-smoothed fabric tensor (local structural anisotropy) that is calculated using SALSA. For detailed information of the fabric tensor calculation, see the section of SALSA derivation. As shown in Fig. 15, we ﬁnd that both the pressure and shear stress ﬂuctuations are evenly distributed throughout the polycrystal. This is in sharp contrast to simulation results of sheared atomic polycrystals [14], which showed much stronger virial ﬂuctuations at grain boundaries than in grain interiors.

30

30 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION

[1] John F Brady. The rheological behavior of concentrated colloidal dispersions. J. Chem. Phys., 99(July):567–581, 1993. [2] Jean-Pierre Hansen and Ian R McDonald. Theory of simple liquids. Elsevier, 1990. [3] Erik Lange, Jose B Caballero, Antonio M Puertas, and Matthias Fuchs. Comparison of structure and transport properties of concentrated hard and soft sphere ﬂuids. The Journal of chemical physics, 130(17):174903, 2009. [4] David R Foss and John F Brady. Brownian dynamics simulation of hard-sphere colloidal dispersions. Journal of Rheology (1978-present), 44(3):629–651, 2000. [5] WCK Poon. The physics of a model colloid–polymer mixture. Journal of Physics: Condensed Matter, 14(33):R859, 2002. [6] D Rosenbaum, PC Zamora, and CF Zukoski. Phase behavior of small attractive colloidal particles. Physical review letters, 76(1):150, 1996. [7] VERONIQUE Trappe, V Prasad, Luca Cipelletti, PN Segre, and DAVID A Weitz. Jamming phase diagram for attractive particles. Nature, 411(6839):772–775, 2001. [8] Klaus Zahn, Axel Wille, Georg Maret, Surajit Sengupta, and Peter Nielaba. Elastic properties of 2d colloidal crystals from video microscopy. Physical review letters, 90(15):155506, 2003. [9] Anand Yethiraj and Alfons van Blaaderen. A colloidal model system with an interaction tunable from hard sphere to soft and dipolar. Nature, 421(6922):513–517, 2003. [10] Kerstin N Nordstrom, E Verneuil, PE Arratia, Anindita Basu, Zheng Zhang, Arjun G Yodh, Jerry P Gollub, and Douglas J Durian. Microﬂuidic rheology of soft colloids above and below jamming. Physical review letters, 105(17):175701, 2010. [11] Ke Chen, Wouter G Ellenbroek, Zexin Zhang, Daniel TN Chen, Peter J Yunker, Silke Henkes, Carolina Brito, Olivier Dauchot, Wim Van Saarloos, Andrea J Liu, et al. Low-frequency vibrations of soft colloidal glasses. Physical review letters, 105(2):025501, 2010. [12] TJ Delph. Local stresses and elastic constants at the atomic scale. Proceedings of the Royal Society A: Mathematical, Physical and Engineering Science, 461(2058):1869–1888, 2005. [13] V. a. Levashov, J. R. Morris, and T. Egami. Viscosity, Shear Waves, and Atomic-Level Stress- Stress Correlations. Phys. Rev. Lett., 106(11):115703, March 2011. [14] Jakob Schiøtz, Francesco D Di Tolla, and Karsten W Jacobsen. Softening of nanocrystalline

31

NATURE MATERIALS | www.nature.com/naturematerials 31 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

metals at very small grain sizes. Nature, 391(6667):561–563, 1998. [15] Ellad B Tadmor and Ronald E Miller. Modeling materials: continuum, atomistic and multi- scale techniques. Cambridge University Press, 2011. [16] AI Murdoch and D Bedeaux. Continuum equations of balance via weighted averages of mi- croscopic quantities. Proceedings of the Royal Society of London A: Mathematical, Physical and Engineering Sciences, 445(1923):157–179, 1994. [17] A Ian Murdoch. A critique of atomistic deﬁnitions of the stress tensor. Journal of Elasticity, 88(2):113–140, 2007. [18] Robert J Hardy. Formulas for determining local properties in molecular-dynamics simulations: Shock waves. The Journal of Chemical Physics, 76(1):622–628, 1982. [19] Ted Belytschko, Yury Krongauz, Daniel Organ, Mark Fleming, and Petr Krysl. Meshless methods: an overview and recent developments. Computer methods in applied mechanics and engineering, 139(1):3–47, 1996. [20] See-Eng Phan, William B Russel, Zhengdong Cheng, Jixiang Zhu, Paul M Chaikin, John H Dunsmuir, and Ronald H Ottewill. Phase transition, equation of state, and limiting shear viscosities of hard sphere dispersions. Physical Review E, 54(6):6633, 1996. [21] Xiang Cheng, Jonathan H McCoy, Jacob N Israelachvili, and Itai Cohen. Imaging the microscopic structure of shear thinning and thickening colloidal suspensions. Science, 333(6047):1276–9, September 2011. [22] Neil YC Lin, Sushmit Goyal, Xiang Cheng, Roseanna N Zia, Fernando A Escobedo, and Itai Cohen. Far-from-equilibrium sheared colloidal liquids: Disentangling relaxation, advection, and shear-induced diﬀusion. Physical Review E, 88(6):062309, 2013. [23] Alejandro Torres-S´anchez, Juan M Vanegas, and Marino Arroyo. Examining the mechan- ical equilibrium of microscopic stresses in molecular simulations. Physical review letters, 114(25):258102, 2015. [24] Colin JR Sheppard, Min Gu, Keith Brain, and Hao Zhou. Inﬂuence of spherical aberration on axial imaging of confocal reﬂection microscopy. Applied optics, 33(4):616–624, 1994. [25] Colin JR Sheppard and Min Gu. Aberration compensation in confocal microscopy. Applied optics, 30(25):3563–3568, 1991. [26] P T¨or¨ok, SJ Hewlett, and P Varga. The role of specimen-induced spherical aberration in confocal microscopy. Journal of microscopy, 188(2):158–172, 1997.

32

32 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.

DOI: 10.1038/NMAT4715 SUPPLEMENTARY INFORMATION

[27] Thijs Herman Besseling, Jissy Jose, and A BLAADEREN. Methods to calibrate and scale axial distances in confocal microscopy as a function of refractive index. Journal of microscopy, 257(2):142–150, 2015. [28] Neil YC Lin, Jonathan H McCoy, Xiang Cheng, Brian Leahy, Jacob N Israelachvili, and Itai Cohen. A multi-axis confocal rheoscope for studying shear ﬂow of structured ﬂuids. Review of Scientiﬁc Instruments, 85(3):033905, 2014. [29] Peter J Shaw and David J Rawlins. The point-spread function of a confocal microscope: its measurement and use in deconvolution of 3-d data. Journal of Microscopy, 163(2):151–165, 1991. [30] Wilson CK Poon, Eric R Weeks, and C Patrick Royall. On measuring colloidal volume fractions. Soft Matter, 8(1):21–30, 2012. [31] Rei Kurita, David B Ruﬀner, and Eric R Weeks. Measuring the size of individual particles from three-dimensional imaging experiments. Nature communications, 3:1127, 2012. [32] Sander Pronk and Daan Frenkel. Large diﬀerence in the elastic properties of fcc and hcp hard-sphere crystals. Physical review letters, 90(25):255501, 2003. [33] Wolfgang Lechner and Christoph Dellago. Defect interactions in two-dimensional colloidal crystals: vacancy and interstitial strings. Soft Matter, 5(14):2752–2758, 2009. [34] Wolfgang Lechner and Christoph Dellago. Point defects in two-dimensional colloidal crystals: simulation vs. elasticity theory. Soft Matter, 5(3):646–659, 2009. [35] Fabio Cinti, Tommaso Macr`ı,Wolfgang Lechner, Guido Pupillo, and Thomas Pohl. Defect- induced supersolidity with soft-core bosons. Nature communications, 5, 2014. [36] CH Bennett and BJ Alder. Studies in molecular dynamics. ix. vacancies in hard sphere crystals. The Journal of Chemical Physics, 54(11):4796–4808, 1971. [37] Peter Schall, Itai Cohen, David A Weitz, and Frans Spaepen. Visualization of dislocation dynamics in colloidal crystals. Science, 305(5692):1944–1948, 2004. [38] Derek Hull and David J Bacon. Introduction to dislocations, volume 37. Elsevier, 2011. [39] Alexander Stukowski and Karsten Albe. Extracting dislocations and non-dislocation crystal defects from atomistic simulation data. Modelling and Simulation in Materials Science and Engineering, 18(8):085001, 2010. [40] ML Falk and JS Langer. Dynamics of viscoplastic deformation in amorphous solids. Physical Review E, 57(6):7192, 1998.

33

NATURE MATERIALS | www.nature.com/naturematerials 33 © 2016 Macmillan Publishers Limited. All rights reserved.

SUPPLEMENTARY INFORMATION DOI: 10.1038/NMAT4715

[41] Daan Frenkel and Anthony JC Ladd. Elastic constants of hard-sphere crystals. Physical review letters, 59(10):1169, 1987. [42] Valentin A Levashov, James R Morris, and Takeshi Egami. Viscosity, shear waves, and atomic- level stress-stress correlations. Physical review letters, 106(11):115703, 2011. [43] C Mottet, G Rossi, F Baletto, and R Ferrando. Single impurity eﬀect on the melting of nanoclusters. Physical review letters, 95(3):035501, 2005. [44] Kenji Yoshimoto, Tushar S Jain, Kevin Van Workum, Paul F Nealey, and Juan J de Pablo. Mechanical heterogeneities in model polymer glasses at small length scales. Physical review letters, 93(17):175501, 2004. [45] There is a nomenclature problem when describing the stress and strain around a point defect. Some describe them as quadrupolar ﬁelds, reﬂecting the similar cos 2θ angular dependence with electrical quadrupoles. This angular dependence is special, however, to isotropic elastic theory; also, the displacement ﬁeld has a ‘monopolar’ isotropic component ∆V/(4πr2) with no angular dependence. (However, as noted in Fig. 3, the oﬀ-diagonal stresses for an isotropic vacancy still look like quadrupoles.) Some describe them as elastic dipoles, reﬂecting both the common 1/r3 force law with electric dipoles and their origins as ‘force dipoles’ (two opposite forces acting on nearby points in the elastic medium.) Finally, others (particularly studying elasticity in amorphous systems) name the ﬁeld after Eshelby – thus bypassing the choice by using an uninformative label. Here, we use the term quadrupole, mostly because the ‘strength’ of a point defect is quantiﬁed by a 3x3 symmetric matrix (either the strain

quadrupole Qij described here, or the corresponding stress quadrupole / force dipole.) We

must note, however, that in the present case of vacancies in a cubic environment, Qij =∆Vδij has no correspondence to electric quadrupoles, which are traceless.

34

34 NATURE MATERIALS | www.nature.com/naturematerials © 2016 Macmillan Publishers Limited. All rights reserved.